Extending the supramolecular synthon based fragment approach (SBFA) for transferability of multipole charge density parameters to monofluorobenzoic acids and their cocrystals with isonicotinamide: importance of C-H···O, C-H···F, and F···F intermolecular regions.
Hathwar, Venkatesha R.; Thakur, Tejender S.; Dubey, Ritesh; Pavan, Mysore S.; Row, Tayur N Guru; Desiraju, Gautam R.; The journal of physical chemistry. A 115 (2011) 12852–12863; doi:10.1021/jp2039866

data_1516189
_publ_section_title
;
 Extending the supramolecular synthon based fragment approach (SBFA) for
 transferability of multipole charge density parameters to
 monofluorobenzoic acids and their cocrystals with isonicotinamide:
 importance of C-H&#x00B7;&#x00B7;&#x00B7;O, C-H&#x00B7;&#x00B7;&#x00B7;F,
 and F&#x00B7;&#x00B7;&#x00B7;F intermolecular regions.
;
_journal_issue                   45
_journal_name_full               'The journal of physical chemistry. A'
_journal_page_first              12852
_journal_page_last               12863
_journal_paper_doi               10.1021/jp2039866
_journal_volume                  115
_journal_year                    2011
_chemical_compound_source        'see text'
_chemical_formula_sum            'C7 H5 F O2'
_chemical_formula_weight         280.22
_chemical_name_common            '4-Flurobenzoic acid'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 94.353(18)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.816(6)
_cell_length_b                   6.3759(11)
_cell_length_c                   26.571(4)
_cell_measurement_reflns_used    4610
_cell_measurement_temperature    293
_cell_measurement_theta_max      27.8
_cell_measurement_theta_min      3.1
_cell_volume                     644.6(10)
_computing_cell_refinement
;
CrystalClear-SM Expert 2.0 rc14 (Rigaku, 2009)
;
_computing_data_collection
;
CrystalClear-SM Expert 2.0 rc14 (Rigaku, 2009)
;
_computing_data_reduction
;
CrystalClear-SM Expert 2.0 rc14 (Rigaku, 2009)
;
_computing_publication_material  'PLATON (Spek, 2003)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293
_diffrn_detector_area_resol_mean 13.6612
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_details
;
scan:
    Number of images: 360
               Slice: -60.0000 - 120.0000
         Image width: 0.5000
            Exp time: 10.0000
       Rotation axis: Omega
               Omega: 0.0000
                 Chi: 54.0000
                 Phi: 0.0000
                 XTD: 49.4000
              2theta: 29.6000
scan:
    Number of images: 360
               Slice: -60.0000 - 120.0000
         Image width: 0.5000
            Exp time: 10.0000
       Rotation axis: Omega
               Omega: 0.0000
                 Chi: 54.0000
                 Phi: 120.0000
                 XTD: 49.4000
              2theta: 29.6000
scan:
    Number of images: 360
               Slice: -60.0000 - 120.0000
         Image width: 0.5000
            Exp time: 10.0000
       Rotation axis: Omega
               Omega: 0.0000
                 Chi: 54.0000
                 Phi: 240.0000
                 XTD: 49.4000
              2theta: 29.6000

;
_diffrn_measurement_device
;
XtaLABmini: Fixed Chi 2 circle
;
_diffrn_measurement_device_type
;
Rigaku Mercury375R (2x2 bin mode)
;
_diffrn_measurement_method       'profile data from \w-scans'
_diffrn_orient_matrix_type       FS_PROCESS
_diffrn_orient_matrix_UB_11      0.069456
_diffrn_orient_matrix_UB_12      0.045183
_diffrn_orient_matrix_UB_13      0.034058
_diffrn_orient_matrix_UB_21      -0.252274
_diffrn_orient_matrix_UB_22      0.026962
_diffrn_orient_matrix_UB_23      -0.257871
_diffrn_orient_matrix_UB_31      0.024796
_diffrn_orient_matrix_UB_32      0.147751
_diffrn_orient_matrix_UB_33      0.036642
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'Sealed Tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0438
_diffrn_reflns_av_sigmaI/netI    0.0362
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            5658
_diffrn_reflns_theta_full        27.52
_diffrn_reflns_theta_max         27.52
_diffrn_reflns_theta_min         3.08
_exptl_absorpt_coefficient_mu    0.124
_exptl_absorpt_correction_T_max  0.994
_exptl_absorpt_correction_T_min  0.958
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Jacobson, R. (1998) Private communication'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    1.444
_exptl_crystal_density_method    'Not Measured'
_exptl_crystal_description       Plate
_exptl_crystal_F_000             288
_exptl_crystal_size_max          0.350
_exptl_crystal_size_mid          0.300
_exptl_crystal_size_min          0.050
_refine_diff_density_max         0.138
_refine_diff_density_min         -0.134
_refine_diff_density_rms         0.034
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     111
_refine_ls_number_reflns         1464
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.043
_refine_ls_R_factor_all          0.0806
_refine_ls_R_factor_gt           0.0546
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0521P)^2^+0.0688P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1141
_refine_ls_wR_factor_ref         0.1254
_reflns_number_gt                979
_reflns_number_total             1464
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            4fbza293kplaton.cif
_cod_data_source_block           shelxl
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/usr/data/users/saulius/automatic-downloads/retrospective/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               1516189